Gear Failure Analysis - Gear Failure Analysis Author: Sandy Polak Subject: Investigation of Gear...
Embed Size (px)
Transcript of Gear Failure Analysis - Gear Failure Analysis Author: Sandy Polak Subject: Investigation of Gear...
Neale Consulting Engineers Ltd The Tribology Handbook www.tribology.co.uk
4.1 Gear failures
Gear failures rarely occur. A gear pair has not failed until it can no longer be run. This condition is reached when (a) one or more teeth have broken away, preventing transmission of motion between the pair or (b) teeth are so badly damaged that vibration and noise are unacceptable when the gears are run.
By no means all tooth damage leads to failure and immediately it is observed, damaged teeth should be examined to determine whether the gears can safety continuein service.
This includes case exfoliation in skinhardened gears and pitting which is the commonest form of damage, especially with unhardened gears. Pitting, of which four types are distinguished is indicated by the development of relatively smoothbottomed cavities generally on or below the pitch line. In isolation they are generally conchoidal in appearance but an accumulation may disguise this.
Case exfoliation Characteristics
Appreciable areas of the skin on surface hardened teeth flake away from the parent metal in heavily loaded gears.Carburised and hardened, nitrided and induction hardened materials are affected.
Case exfoliation often indicates a hardened skin that is too thin to support the tooth load. Cracks sometimes originate on the plane of maximum Hertzian shearstress and subsequently break out to the surface, but more often a surface crack initiates the damage. Anotherpossible reason forcase exfoliation is the high residual stress resulting from too severe a hardness gradient between case and core. Exfoliation may be prevented by providing adequate case depth and tempering the gearmaterial afterhardening.
Case exfoliation on a spiral bevel pinion
Initial or arrested pitting
Initial or arrested pitting on a single helical gear
Initial pitting usually occurs on gears that are not skin hardened. It may be randomly distributed over the whole tooth flank, but more often is found around the pitch line or in the dedendum. Single pits rarely exceed 2mm across and pitting appears in the early running life of a gear.
Discrete irregularities Iprofile orsurface asperities are subjected to repeated overstress as the line of contact sweeps across a tooth to produce small crack and clefts. In the dedendum area the oil under the high pressure of the contact can enter these defects and extend then little by little, eventually reaching the surface again so that a pit is formed and a small piece of metal is dislodged. Removal of areas of overstress in this way spreads the load on the teeth to a level where further crack or cleft formation no longeroccurs and pitting ceases.